Presentation on theme: "Second International Conference on Innovative Natural Fibre Composites for Industrial Applications Stanislaw Kuciel, Aneta Liber-Knec Biocomposites on."— Presentation transcript:
Second International Conference on Innovative Natural Fibre Composites for Industrial Applications Stanislaw Kuciel, Aneta Liber-Knec Biocomposites on the Base of Thermoplastic Starch Filled by Wood and Kenaf Fiber Tadeusz Kościuszko Cracow University of Technology Division of Experimental Mechanics and Biomechanice - POLAND April 15-18, 2009, Rome KEYWORDS: Thermoplastic starch, Mechanical & physical properties, Reinforcements
plastics from renewable resources The increasing danger for the environment and people health connected with plastics wastes turned researches attention to plastics from renewable resources which have properties similar to petrochemical polymers but can be biodegradable Biopolymers are very often used to combine with natural fiber as well a being a part of biodegradable synthetic plastics In recent years, among the functional fillers, natural fibres have become a common material for the manufacture of filled plastics.
biocomposites made of thermoplastic starch were tested to estimate the influence of the wooden or kenaf filler on their based physical and mechanical properties influence of using two sorts of thermoplastic biobased and biodegradable starch was also estimated Biocomposites properties (physical, mechanical) were estimated on the basis of several tested including also influence of themperature and soaking in the water the reinforcement effect was estimated by making SEM micrographs of surface (fractures and polished cross-sections), RESARCHE PROGRAMME: Conclusions from the results of tests let to propose and make some products based on thermoplastic starch with natural fillers
BIOBASED THERMOPLATIC STARCH ON MATRIX OF COMPOSITE Solanyl BP blend 20F (potato starch) – S2 Solanyl BP blend 30R (potato starch) – S3 produced by Rodenburg Biopolymers from the Netherlands. Solanyl® BP is a patented and comercially available bioplastic, a smart material which is biobased and biodegradable. The word Solanyl is coming from Solanum Tuberosum, which means potato. Polymer is based on a side stream potato starch of the potato processing industry. Production of Solanyl granules is highly efficiently and for example requires 65% less energy compared to polyethylene production.
FILLERS: CB 120 100x The specific shape of wooden (pink) filler manufactured by Retttenmajer Lignocel CB 120 WOOD FIBER – produced by J.Rettenmaier & Söhne Co which worked out family of wooden fillers for filling polymer composites known as trade name Lignocel®. The wood fibre CB 120 is produced from pine, has fibrous structure and the length of particles is about 70-150 m. Lignocel is natural fiber which is “ready-to-use“ for direct processing on extrusion plants and injection molding machinery
KENAF FIBER The kenaf fiber deriving from processing the bark of the kenaf plant is pale yellow in color and is the most highly valued natural product. It has a degree of purity from woody debris and pectins equal to 99% and is highly appreciated in the construction of mats with thermoset natural fibres for the automotive industry and technical applications. The fibers after grinding in our laboratory on Retsch mill machine have approximately 40- 50 μm and length 200-300 μm. produced by Kenaf Eco Fibers Italy
Scanning electron micrographs (SEM) of the sisal fiber Lignocel ® CB 120 Scanning electron micrographs (SEM) of the wood fiber Scanning electron micrographs (SEM) of the flax - len
SEM micrographs of: (a)-surface of composite with 20% wood fibres (fracture, x1000) (b) “Channels” of wood fibres filled by polymer (polished cross-section, x500) a) b)
COMPARABLE FIBRE CHARACTERISTICS B. COMMON CHARACTERISTICS - PHYSICAL High tensile strength Low extension High modulus of elasticity High coefficient of friction Excellent heat, sound, electrical insulation properties Biodegradable Combustible C.COMMON CHARACTERISTICS - COMMERCIAL Abundant global supply Renewable, sustainable raw material resource Recyclability Potential for comparable weight reduction Potential for comparable cost reduction
5-40 % wood filled profiles basically conventional equipment; stiffness, marble effects twin (also parallel) or single 40-70 % wood like profiles Strandex or similar (USA: decking market) conical machines 70-90 % wooden profiles outside, construction, high stiffness, image conical machines 60+20 % and higher Fasalex MDF, interior, image, 100% organic feasible conical machines Calibration Water cooling No Calibration Air cooling Possibilities of processing
Specimens Specimens were made according to EN ISO 527-2 using injecting-moulding machine Wh80 Ap with double mold form at laboratory of University of Technology and Life Sciences - Bydgoszcz (Poland). Additionally, for preparing and better homogenization of Solanyl granulates with the fillers, there was used roll stand machine (roll length – 380 mm and diameter – 200 mm) for making composites. The rolling was conducted in the temperature of 160 °C. Then granulated fraction was injected. The weight content of fibers in composites was 25 and 40% of wood and kenaf fibers (specimens indicated 25C, 4C and 25K, 4K).
The injection-molded tensile bars were tested at 21°C and 65% RH on a universal testing instrument (Instron type 4465) according to PN-EN ISO 527. Using a constant crosshead speed of 5 mm/min, five tensile bars were tested for each composite and the mean and range of the specific modulus of elasticity, specific ultimate tensile strength and strain at break. Type of biopolymerwt of fibre [%]Density [g/cm 3 ] Solanyl 20F 0 1.2997 Solanyl 20F 25 wood 1.3270 Solanyl 20F 40 wood 1.3413 Solanyl 20F 25 kenaf 1.3275 Solanyl 20F 40 kenaf 1.3522 Solanyl 30R 0 1.3040 Solanyl 30R 25 wood 1.3388 Solanyl 30R 40 wood 1.3500 Solanyl 30R 25 kenaf 1.3342 Solanyl 30R 40 kenaf 1.3546
Results of tests: The influence of the filler Comparison of modulus of elasticity for tested composites (C - wood, K – kenaf)
Comparison of tensile strenght for tested composites (C - wood, K – kenaf) In case of biopolymers filled by kenaf fibers, the values of modulus of elasticity and tensile strength are higher than for wood fibre composites, but processing composites with kenaf is more difficult.
SEM image Solanyl BP 20F, fragile fracture after break in liquid N2 Solanyl BP 30R, fracture after elongation test with pulled out elements of thermoplastic starch JEOL 5510LV (low vacuum) scanning electron microscope (SEM) with an accelerating voltage of 10 kV It`s interesting that producer used two form of granulate: one of them is more stiffness and harder, melts in higher temperature and another one is more plastificate and easy melting
single wood fiber in polymeric matrix – Solanyl 20F with 25% of fiber, fracture after elongation test kenaf fiber broken during elongation test, fracture Solanyl 30R filled by 40% of fiber We can observe the differences between morphology of chosen natural fiber – kenaf fiber seems be more coherent but both has good adhesion to thermoplastic starch
typical fracture of composite on the base of Solanyl 30R filled by 40% with characteristic shapes of wood fiber, cross section after breaking in elongation test. typical fracture of composite on the base of Solanyl 30R (with two phase matrix of biopolymer) filled by 40% of kenaf fiber (observed like second phase) fracture after elongation test This stress transfer efficiency largely depends on the fiber- matrix interface and mechanical properties of the fiber and polymer
Absorption of water - first effect of biodegradation Comparison of absorption of water for composition with kenaf (K) and wood fiber (C) on the base of two sorts of thermoplastic starch on trade name - Solanyl We can observe that adding wood and kenaf fibres caused increase of absorbed water by composites. The values of absorbed water for composites with wood fibre and on the base of Solanyl 30R are higher
Examples of elongation curves for Solanyl 20F and wood fibre (dry and soaked 7 days in water – W7)
Type of biopolymer wt of fibre [%] Proportional decrease of the following values for wet specimens (after 7 days) compared to dry Tensile strenght [%]Modulus of elasticity [%] Solanyl 20F01.66.2 Solanyl 20F25 wood14.07.3 Solanyl 20F40 wood19.028.5 Solanyl 20F25 kenaf8.87.4 Solanyl 20F40 kenaf31.733.9 Solanyl 30R028.831,3 Solanyl 30R25 wood36.717.5 Solanyl 30R40 wood27.441.0 Solanyl 30R25 kenaf20.125.5 Solanyl 30R40 kenaf20.729.7
Comparison of modulus of elasticity for Solanyl 20F and wood fiber tested in three temperatures When a polymer specimen is tension tested at elevated temperatures, its modulus and strength decrease with increasing temperature because of thermal softening. In a polymeric matrix composite, the matrix-dominated properties are more affected by increasing temperature than the fiber-dominated properties
Comparison of tensile strength for Solanyl 20F and wood fiber tested in three temperatures
Comparison of modulus of elasticity for Solanyl 30R and wood fiber tested in three temperatures The increase of temperature of testing caused decrease of tensile strength and modulus and elongation increased. In case of composite with 40 % of kenaf fiber tested in 60°C, elongation was about 62 mm.
Comparison of tensile strength for Solanyl 30R and wood fiber tested in three temperatures
Conclusions Biocomposites on the base of thermoplastic starch filled by natural fibers, both from renewable material, can be interested alternative for conventional polymeric material based on gas or oil modified hand-mad fiber like glass or carbon. We can examine that this composites can obtain strength on the level 50 MPa and very good stiffness with modulus of elasticity coming to 10.000 MPa. Polymer composites on thermoplastic starch filled with kenaf had highest increase of stiffness on the same level of fiber than composites on the base of polyolefines. On the fracture images, we can observe regular distribution of the fibres in the matrix and two-phase character of the starch matrix.
It seems that we can process this biocomposietes on classical plastic machine like injection-moulding machine or conventional extruders. It is important that we can used less electric energy with the same efficiency of processing because melting temperature of based thermoplastic starch is lower than polyolefin’s or other traditional plastic (PCV, PS or PA). Soaking in the water especially for longer time and higher temperature caused decreasing of mechanical properties and this is a opportunity for some technical application but it isn’t a problem for many every-day product with short time life cycle. At the U.S. Department of Agriculture (USDA) laboratories and elsewhere, research on starch polymers has focused on several areas including utilizing, commodity starches in foams, composites, building materials, adhesive and blends Conclusions
Division of Experimental Mechanics and Biomechanics ul. Jana Pawła II 37, 31-864 Kraków, POLONIA Invitare per Cracovia! Contakt: Stanisław KUCIEL - firstname.lastname@example.org Aneta LIBER-KNEC - email@example.com